Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

- Springer handbook of nanomaterials by Springer 1515 views
- Field flow fractionation in biopoly... by Springer 678 views
- Theory of electroelasticity by Springer 805 views
- Polymer physics by Springer 534 views
- Chemical identification and its qua... by Springer 785 views
- Higher oxidation state organopallad... by Springer 939 views

1,207 views

Published on

No Downloads

Total views

1,207

On SlideShare

0

From Embeds

0

Number of Embeds

8

Shares

0

Downloads

0

Comments

0

Likes

3

No embeds

No notes for slide

- 1. Struct Bond (2011) 138: 31–66 DOI: 10.1007/430_2010_34 # Springer-Verlag Berlin Heidelberg 2010 Published online: 3 December 2010 Crystal Structures of Inorganic Oxoacid Salts Perceived as Cation Arrays: A Periodic-Graph Approach Vladislav A. Blatov Abstract A total of 569 crystal structures of anhydrous simple salts My(LO3)z (L ¼ B, C, N, S, Se, Te, Cl, Br, I) and My(XO4)z (X ¼ Si, Ge, P, As, S, Se, Cl, Br, I) are considered as three-periodic nets of My(L/X)z, where M are cations derived from metal atoms whereas (L/X) are conventional cations derived from nonmetal atoms. Both L and X cations are located in the centers of triangular/trigonal- pyramidal LO3 and tetrahedral XO4 oxoanions, respectively. The cation arrays (MþL/X) are proved to be the elements determining and governing the topology of the respective crystal structures, whereas the oxygens seem to play a secondary role as links between the cations. The preponderant role of cations in determining the crystal structures is founded on a greater uniformity (regularity) of their arrays when compared with those of anions or, even, with mixed cation–anion arrange- ments. In about three-fourth of the crystal structures analyzed in this work, the cation arrays appear to be topologically equivalent to some binary compounds, such as NaCl, NiAs, FeB, and a-Al2O3. The inﬂuence of both charge and size on the resulting array topology is also studied in detail. A quasi-binary representation My[L/X]z is proposed as a general model for the crystal structures of these anhy- drous oxoacid salts. Keywords Cation arrays, Ionic packings, Oxoacid salts, Periodic graph, Software and databases Contents 1 Introduction ................................................................................ 32 2 Periodic-Graph Approach in Crystal Chemistry ........................................... 33 2.1 Terminology ......................................................................... 33 2.2 The Concepts of Structure Representation, Underlying Net, and Packing Net ...... 37 2.3 Computer Tools to Study Periodic Graphs ........................................... 40 V.A. Blatov Samara State University, Ac. Pavlov St. 1, Samara 443011, Russia e-mail: blatov@ssu.samara.ru
- 2. 3 Underlying Nets and Cation Arrays in Inorganic Oxoacid Salts ........................... 41 3.1 Oxoacid Salts with Triangular Anions ............................................... 41 3.2 Oxoacid Salts with Trigonal-Pyramidal Anions ..................................... 48 3.3 Oxoacid Salts with Tetragonal Anions ............................................... 52 3.4 Uniformity of Cation Arrays in Inorganic Oxoacid Salts ............................ 59 4 General Regularities in the Cation Arrays ................................................. 60 5 Concluding Remarks ....................................................................... 62 References ......................................................................................63 1 Introduction Those crystal structures with a pronounced ionic bonding have represented a good ﬁeld for exploring crystallochemical models and theories. Since the very beginning, two of these models have become widely used and commonly accepted. Usually, ions are considered to have well-deﬁned sizes of approximate spherical shape that can be described within a simple geometrical model of sphere packing. Since the Coulomb forces are nondirectional, one can apply a model of point charges being in equilibrium. Both models postulate that one ionic component (cations or anions) determines the structure pattern, while the other component plays a subordinate role following the structure-forming component and introducing only slight modiﬁcations in the “ideal” skeleton. However, the roles of the components can be quite different in the two models. In most tables of ionic radii, anions are larger than cations, so that the ﬁrst model ordinarily represents the ionic crystal as packing of anions with cations occupying the packing holes. In contrast, the second model considers cations as the structure-forming component since they usually have larger effective charges than anions. The model of sphere packing is the oldest one in crystal chemistry and is commonly used for description of inorganic ionic compounds even nowadays. In 1972, Lebedev [1] stressed the priority of connections between cations, in particular, in the rutile crystal structure. Then, O’Keeffe and Hyde, in a series of publications [2–4], drew attention to the fact that many ionic crystals can be considered as regular arrays of cations, while anions play a subordinate role (oxygen-stuffed alloys). The regular arrangement of cations was called eutactic [2] to emphasize that although the centers of cations often occupy the positions of a regular packing, the cations do not touch each other. Borisov [5] showed that the structure types of heavy-cation oxides, ﬂuorides, and sulﬁdes are determined by the cation arrays densely packed into almost planar layers. In many cases, the cation array in complex oxides reproduces the structure of simple intermetallic or ionic compounds with the same stoichiometry. In both cases, however, oxygens are considered as a medium and the complex oxide can be treated as an “anion-stuffed alloy” [4]. For instance, the cation array Ca2Si in larnite (b-Ca2SiO4) is arranged like d-Ni2Si where a main metallic bonding is assumed [4]. On the contrary, the sodium and sulfur cations in Na2SO4 adopt the structure of an ionic compound like the high-pressure phase of Na2S [6]. 32 V.A. Blatov
- 3. Many other examples of such similarities are collected in [7] and a brief consider- ation of inorganic oxysalts as cation arrays can be found in [8]. O’Keeffe and Hyde [3, 4] illustrated the eutaxy by many examples and consid- ered this phenomenon as a result of mutual repulsion of cations. Further attempts to interpret these experimental facts were undertaken by Vegas et al. [6, 7, 9–12], by extending the Zintl–Klemm concept to the cation arrays in oxides. It should be recalled that the original Zintl concept [13] was conceived to explain the crystal structures of compounds formed between highly electropositive atoms (A) and main-group atoms (X). The resulting structure consists of an X-skeleton in which the X atoms are bonded by directed covalent bonds, whose connectivity obey the 8-N rule (where N is the number of valence electrons of X). In this type of compounds (the so-called Zintl-phases), it is assumed that all valence electrons of the A atoms are formally transferred to the X atoms, forming so a negatively charged X-skeletons known as Zintl polyanions. Because the X-skeletons adopt the structure of the element, whose number of electrons is equal to N plus the electrons transferred from A, Klemm [14] named the X atoms as pseudo-atoms. Vegas [7] extended the Zintl–Klemm concept to oxides with complex oxoanions [XOn] and rationalized the structures of many ionic compounds. The cation array model was then developed in [15–17] by applying the concept of an inﬁnite graph (net), which allows one to formally describe the cation arrays and to analyze their geometrical-topological properties with strict computer algo- rithms. Using the program package TOPOS [18], we studied topological motifs in all known crystal structures of inorganic salts of formulae My[LO3]z or My[XO4]z. In them, the [LO3] groups have either trigonal or trigonal-pyramidal geometry, and the [XO4] oxoanions are tetrahedral. The study revealed that more than 50% of the structures followed the motifs of binary compounds AyXz. The eutaxy of those arrays was evaluated by numerical criteria of uniformity, based on the Voronoi partition of the crystal space. Our aim, in this chapter, is to extend the analysis of the cation arrays, using novel methods of crystal structure taxonomy. These methods are based on the concept of underlying net derived from the periodic-graph approach and have been initially developed to explore metal-organic frameworks [19]. We will show the general applicability of these new tools that can be easily adjusted to describe the crystal structures of any composition and bonding type. 2 Periodic-Graph Approach in Crystal Chemistry 2.1 Terminology The term “topology” is often used in chemistry rather ambiguously [20]. Although in most cases the crystal chemists admit that topology describes the properties of connectivity of the crystal space, even the assertion that “the structures are Crystal Structures of Inorganic Oxoacid Salts 33
- 4. topologically equal (similar, different) to. . .” is usually drawn after a visual analy- sis, comparing only a few local topological properties of the structures, while the overall structure topology is the natural crystallochemical subject. In short, crystal chemistry begins when the crystal structure topology is taken into consideration. Below, we brieﬂy consider the simplest formalization of the crystal space topology perceived as a periodic graph. A more detailed terminology on this topic can be found in [21]. Graph is a set of vertices (points); each ordered pair of the vertices determines an edge of the graph. The set of all edges is called the topology of the graph. Since in crystal chemistry the graph vertices and edges correspond to atoms and interatomic bonds, respectively, the chemical term “topology” means merely the set of all interatomic bonds in the crystal structure. Net is a kind of inﬁnite graph that is simple (it has no loops, multiple or directed edges) and connected (any pair of vertices in the graph is connected by a chain of edges); vertices of the graph are often called nodes of the net. The degree n of a node is the number of edges incident to the node; it is equivalent to coordination number of the corresponding atom, so that the node (atom) is called n-coordinated. A subnet (supernet) of the net A is a net whose sets of nodes and edges are subsets (supersets) of corresponding sets of A. Two nets are called isomorphic if there is one-to-one mapping between the sets of their nodes and edges. The symmetry of the net is described by an automorphism group that enumerates all possible permuta- tions of nodes giving rise to isomorphic nets; this symmetry does not involve any geometrical realization of the net and, hence, can be considered as “topological” symmetry of the corresponding chemical structure. Net is n-periodic if its automor- phism group contains a subgroup being isomorphic to a group of n-independent translations. When we consider some arrangement of the net nodes in the space, we speak about an embedding of the net. The symmetry of the net embedding can be lower (but not higher) than the symmetry of the net. Coordination ﬁgure of the node is the solid formed by nodes incident to this node; if the coordination ﬁgure has a polyhedral form, it corresponds to the coordination polyhedron of the corresponding atom. The net is uninodal (bi-, tri-,. . ., polynodal) if all its nodes are equivalent by symmetry (or there are two, three,. . ., many nonequivalent nodes). If the crystal structures have isomorphic nets, they are called (topologically) isotypic belonging so to the same topological type [22]. Since the notion of isomorphism is strictly determined, the concept of topological type is a way to an objective taxonomy (independent of the visual analysis) of crystal structures. Note that the oldest primary classiﬁcation taxon in crystal chemistry, structure type, arranges crystal structures according to their geometrical properties (unit cell dimensions, space group, atomic positions). In contrast, topological type includes all structures with the same system of chemical bonds irrespective of their embed- dings. To designate the topological type, we can use the name of one of its representatives as well as the symbol of the net corresponding to the type. In this chapter, we will use three kinds of nomenclature for net symbols: (1) three-letter symbols from the RCSR database, (2) sqcXXX EPINET codes (see Sect. 2.3), and 34 V.A. Blatov
- 5. (3) s-d-G-n symbols proposed in [23] for the subnets derived from the most important crystallochemical nets. For example, the RCSR symbols dia (the corresponding EPINET code sqc6) and dia-b are assigned to both the diamond net and the isotypic binary compound (sphalerite, ZnS), with the same topology, but with two chemi- cally and crystallographically nonequivalent atoms. The s-d-G-n symbol nia-5,5- Pna21 designates the subnet derived from the RCSR nia (NiAs) net with two topologically different 5-coordinated atoms, and the maximum-symmetry embed- ding of the net has the space group Pna21. If a net does not fall in any topological classiﬁcation, we designate it by the Cambridge Structural Database Reference Code or by the chemical formula of the corresponding compound. When performing the topological taxonomy, the problem that emerges is how to compare two inﬁnite objects that are periodic nets. The representation of a periodic net as a ﬁnite object is achieved by means of the concept of labeled quotient graph [24]. The labeled quotient graph is a graph whose vertices and edges correspond to inﬁnite sets of both translation-equivalent nodes and edges of the net; the corresponding atoms and bonds occupy the same primitive cell of the crystal structure. Hence, the labeled quotient graph is ﬁnite, but it stores all the information about the net topology. It is extremely important to develop the theory of labeled quotient graphs; this theory could play the same role for crystal chemistry as space- group theory did for crystallography. Such attempts have been undertaken in recent years [25–27]. Topological index of a net is a set of numbers that is related to the net topology. The net topology is completely described by the adjacency matrix of the labeled quotient graph; the adjacency matrix contains the information about all edges (chemical bonds) of the net. Thus, the adjacency matrix can be used as the strictest topological index to check the isomorphism of the nets [28] and also to relate the crystal structures to the same topological type. For a quick comparison of the net topologies or to ﬁnd non-strict topological similarities, one can use other kinds of topological indices [23, 29]. Coordination sequence {Nk} is a set of numbers N1, N2, . . . representing the atoms in the ﬁrst, second, etc., coordination shells around a given atom of the net (Fig. 1). The ﬁrst ten coordination shells are usually consid- ered for the topological classiﬁcation. The cumulative number of atoms in the ﬁrst ten coordination shells averaged over all nonequivalent atoms (TD10) is deﬁned as the topological density of the net; the larger TD10, the denser the net, i.e., the more neighbors are in a local area of the net node. Point symbol lists the shortest circuits (closed chains of connected atoms) meeting at all bond angles of each nonequiva- lent atom in the net. Extended point symbol gives the information on circuits in more detail, while net point symbol summarizes the point symbols for all nonequiv- alent atoms with the corresponding stoichiometric coefﬁcients. Vertex symbol gives the information similar to extended point symbol but for rings (circuits without shortcuts). If the nets have equal sets of all these indices, they are assumed to be topologically isotypic [23]. If the sets of indices are different, but close to each other, the nets can be considered topologically similar. The same can be said of different atoms in the same structure: if their indices are identical, the atoms are topologically equivalent even if they are not related by a space-group operation. Crystal Structures of Inorganic Oxoacid Salts 35
- 6. For example, in the NaCl structure (topological type pcu-b) there are two chemi- cally and crystallographically different atoms, but both Na and Cl are topologically identical since they possess the same set of topological indices (the net point symbol coincides with the point symbols of Na and Cl; Table 1). On the contrary, in NiAs (topological type nia) Ni and As atoms are topologi- cally different, in spite of having similar indices, also close to those of NaCl. In particular, the point symbols of Ni and Na(Cl) are the same {412 .63 }, i.e., in both cases the minimal circuits of bonds are the same (12 fourfold and 3 sixfold circuits). Other nets collected in Table 1 can also be considered as similar to either pcu-b or nia, as it will be discussed below. Fig. 1 Coordination sequence (CS), extended point symbol (ES), point symbol (PS), and vertex symbol (VS) for the uninodal 2-periodic net fes. A 10-circuit is selected that is not a ring (it has a shortcut and composed of two smaller 4- and 8-rings). The nodes of the ﬁrst ﬁve coordination shells are marked by the ordinal number of shell; the initial atom of the sequence formally corresponds to the zero coordination shell Table 1 Topological indices in pcu-b, nia, and related 6-coordinated nets Net (representative) Net point symbol Coordination sequence N1–5 pcu-b (NaCl) {412 .63 } Na, Cl: 6 18 38 66 102 nia (NiAs) {412 .63 }{49 .66 } Ni: 6 20 42 74 114 As: 6 18 42 74 114 sev-6-C2/m (b-HgSeO3) {410 .65 } Hg, Se: 6 19 42 74 115 HIYXUJ (CaSeO3) {410 .65 }{411 .64 } Ca: 6 18 40 70 108 Se: 6 19 40 70 108 FEQWOO (NaIO3) {48 .66 .8}{413 .62 } Na: 6 16 42 72 114 I: 6 20 42 74 114 36 V.A. Blatov
- 7. 2.2 The Concepts of Structure Representation, Underlying Net, and Packing Net While the set of the net nodes is usually predetermined by the chemical composition of the crystal (we do not consider here disordered, incommensurate structures or quasicrystals), the net topology can be established in different ways. The problem of determination of chemical bonding is one of the crucial points of crystallochem- ical analysis. Depending on strength and type of bonding, different sets of bonds can be assigned to the same crystal structure that will have different topologies on the same set of nodes. Moreover, some atoms can be excluded from the analysis if they do not form part of the structure under consideration. 2.2.1 The Concept of Structure Representation One can introduce the concept of (crystal) structure representation as a subset of atoms of the crystal structure as well as some topology speciﬁed on the subset, i.e., any structure representation is a net. Although an inﬁnite number of representations can be ascribed to the same crystal structure, the number of those with crystal- lochemical sense is always ﬁnite and small. For example, one can consider the following representations for the crystal structure of an My(XO4)zÁnH2O oxoacid salt hydrate: (1) the whole structure including H-bonded water molecules, (2) valence-bonded My(XO4)z framework or packing of oxygens with interstitial cations; water molecules as well as H-bonds are ignored, (3) MyXz cation array with direct contacts between ﬁrst-neighbor cations. Note that in this last case, oxygens and their bonds are excluded. The question about which of the several representations is “the best” is meaningless because the goodness depends on the goals of the investigation. All chemically reasonable structure representations can be derived from the so- called complete representation where all atoms and interatomic interactions, even the weakest ones, are taken into account [22]. Any other representation can be obtained from the complete one by some simpliﬁcation procedure. A primary simpliﬁed net can be derived from the complete one by applying the following procedures: (1) removing the edges corresponding to the bonds to be ignored; (2) removing some nodes (atoms) together with their edges (bonds); and (3) contracting some multiatomic groups to their centroids or central atoms but maintaining the structure connectivity. In case (3), all atoms of a multiatomic group are fused in the center of the group giving their bonds to the center; we call this procedure contraction. For instance, the crystal structure of Lu(ClO4)3 (Fig. 2a, see Sect. 3.3.4) can be considered as a net of the Lu atoms and perchlorate anions that are represented by only the Cl atoms after contracting oxygens (Fig. 2b). Thus, the nodes of the primary simpliﬁed net (Lu and Cl) correspond to structural groups of a given chemical compound (the Lu3þ cations and ClO4 – anions), while the nodes of the complete representation always correspond to atoms. Usually the Crystal Structures of Inorganic Oxoacid Salts 37
- 8. primary simpliﬁed net coincides with the so-called standard representation [30], where the structural groups are selected according to a conventional view of the structure. For instance, it is natural to consider the crystal structure of an inorganic oxoacid salt as a framework of metal cations and oxoanions (Fig. 2a). The secondary simpliﬁcation procedure is used if the primary simpliﬁed net contains 0-coordinated Fig. 2 Different representations of the Lu(ClO4)3 crystal structure: (a) all valence bonds are considered; (b) primary simpliﬁed net (standard representation); (c) secondary simpliﬁed net (underlying net); (d) packing net. The Voronoi polyhedron is shown for one of the Lu atoms 38 V.A. Blatov
- 9. (isolated), 1-coordinated (terminal), or 2-coordinated (bridge) nodes; the procedure removes isolated and terminal nodes and contracted bridge nodes converting them into edges as shown in Fig. 2c. 2.2.2 The Concept of Underlying Net After the simpliﬁcation, we obtain an underlying net of the crystal structure [31], i.e., the net that describes the method of connection of the structural groups. If all crystal structures under consideration were simpliﬁed in the same way, their underlying nets can be used to ﬁnd resemblances in their topological organization irrespective of chemical composition, geometrical and topological features of the structural groups. 2.2.3 The Concept of Packing Net The underlying net is derived from the complete representation; so it is always based on the topology of the crystal structure as a whole. This means that edges in this net corresponds to chains of the bonds involving contracted atoms; for instance, the bonds Lu–Lu in Fig. 2b conform to the chains Lu–O–Cl–O–Lu. However, it could be insufﬁcient if the eutaxy of the cation array should be studied since some ﬁrst-neighbor cations in the array could not be linked by such chains. To resolve this problem, we can consider a packing net (cf. [32]), where the edges between the cations are assigned by geometrical, not topological reasons. The assignment criteria could be some range of interatomic distances, or, more precisely, the shape of the Voronoi polyhedra of the cations [32]. In particular, in the Lu cation array of Lu(ClO4)3, there are six additional long (8.11 A˚ ) Lu–Lu contacts (the Voronoi polyhedron of any Lu atom has 6 þ 6 ¼ 12 faces), and the corresponding packing net is f.c.c. (fcu) that allows one to treat the array as a distorted cubic close packing (Fig. 2d). Thus, cation array can be considered as an underlying or packing net; in most cases these nets coincide with each other and, more rarely, the underlying net is a subnet of the packing net. The opposite case (the packing net is a subnet of the underlying net) can occur only in structures with prolonged, not spherical poly- atomic ions [16]. Studying both kinds of net gives the comprehensive and objective information about the topology of the cation array. The approach described above has an important advantage over the traditional visual analysis: it can be made into an algorithm and implemented in a computer program that makes the crystallochemical analysis universal, objective, and fast. With such a program one does not need even to look at the crystal structure; the conclusions about the structure topology, its taxonomy, and comparison with other compounds can be made in an automatic mode. Crystal Structures of Inorganic Oxoacid Salts 39
- 10. 2.3 Computer Tools to Study Periodic Graphs Although the concept of a periodic graph began as far back as the classic series of Wells’ publications [33], the relating computer methods began to develop just in the 1990s. Now there are the following crystallochemical program packages that are based on the periodic-graph approach and distributed free of charge: Gavrog1 consists of two programs: Systre (Symmetry, Structure Recognition, and Reﬁne- ment) [28] is intended to ﬁnd the net embedding with maximal symmetry and to test nets for isomorphism by comparing their adjacency matrices; 3dt (3D tiler) works with 3D space tilings based on periodic nets [34]. TOPOS2 [18] contains a lot of routines to study geometrical and topological properties of crystal structures; it includes the procedures to build various structure representations, underlying and packing nets. Gavrog Systre and TOPOS were used to create a new type of electronic databases that can be called crystallochemical since they describe the topology of periodic nets as contrasted to crystallographic databases like the Cambridge Struc- tural Database or Inorganic Crystal Structure Database that contain the information on atomic positions, perhaps on some bonds, but not on the overall topology of crystal structures. Currently, the following free crystallochemical databases are available: RCSR3 [35] accumulates about 1,800 two- and three-periodic nets of importance for crystal chemistry and selected by hand. Most of them were revealed as underlying nets in crystal structures, and the remaining nets can be useful for crystal design. The three-letter nomen- clature for net topologies used in this chapter was originally elaborated for RCSR. EPINET4 project [36] currently collects 14,532 nets (epinets) generated by special mathematical procedures. Although the epinets do not originate in crystal structures, some of them have been found out as underlying nets. The epinets are denoted by sqcXXX symbols where XXX is an ordinal number, for instance, sqc1964. TTD and TTO collections5 [37] are an integrated part of TOPOS; the TTD collection contains the information on topological indices of more than 71,000 topological types including RCSR and EPINET, while the TTO collection links the data on underlying nets with the structural data stored in crystallographic databases. Below we use the periodic-graph approach together with the TOPOS program package and TTD collection to perform the systematic analysis of topology of cation arrays in inorganic oxoacid salts and to reveal the relations in their structure organization. 1 Generation, Analysis and Visualization of Reticular Ornaments using Gavrog; http://www. gavrog.org. 2 http://www.topos.ssu.samara.ru. 3 Reticular Chemistry Structure Resource, http://rcsr.anu.edu.au/. 4 Euclidean Patterns in Non-Euclidean Tilings, http://epinet.anu.edu.au/. 5 TOPOS Topological Databases and Topological Types Observed, http://www.topos.ssu.samara.ru. 40 V.A. Blatov
- 11. 3 Underlying Nets and Cation Arrays in Inorganic Oxoacid Salts Inorganic oxoacid salts My[LO3]z or My[XO4]z with triangular, trigonal-pyramidal, and tetrahedral anions is a good starting point to demonstrate the advantages of the periodic-graph approach and the concept of underlying net since this class of ionic compounds is numerous (more than 600 crystal structures according to Inorganic Crystal Structure Database, release 2010/1), and the standard representation of their crystal structures is conventional, clear, and simple. The structure units are the cations M and oxoanions [LO3] or [XO4], i.e., oxygens are contracted to L or X cations that represent the anions in the resulting underlying net. Thus, the composition of the underlying net is MyLz or MyXz, i.e., it naturally describes the cation array; the stoichiometric ratio g ¼ y:z is unambiguously determined by charges of the ions. This quasi-binary representation assumes that ionic forces play the most signiﬁcant role in the formation of the periodic structure; the essentially covalent bonding within the anions is considered local and their internal structure is ignored. If the strength of bonds M–O is similar to that of bonds L(X)–O, one can consider the crystal structure of an oxoacid salt as a whole; no simpliﬁcation is applied in this case. The relation to a binary compound can be found if the cations M and L(X) are topologically equivalent; this is so-called grey isomorphism [15]. Vice versa, the existence of “grey isomorphism” could be considered as an implicit indication of similarity of bonding between cations and oxygens in an oxoacid salt; however, this emerges rarely [15–17]. Note that in most cases the authors of original structural investigations do not recognize the relations to binary compounds. We have analyzed 569 crystal structures of oxoacid salts My(LO3)z (L ¼ B, C, N, S, Se, Te, Cl, Br, I) and My(XO4)z (X ¼ Si, Ge, P, As, S, Se, Cl, Br, I), where the underlying nets are 3-periodic. For all of them, the quasi-binary representation was built and the resulting nets were classiﬁed with the TOPOS TTD collection. To characterize the method of coordination of the oxoanion, we use the notation Xmbtk. . . [38], where the letter X shows the ligand denticity (M, B, T, or K for mono-, bi-, tri-, or tetradentate ligands, respectively), the integers mbtk. . . are equal to the numbers of the M atoms connected to one, two, three, or four atoms of the oxoanion. 3.1 Oxoacid Salts with Triangular Anions 3.1.1 Carbonates Carbonates are the most investigated group of the oxoacid salts with triangular anions owing to their signiﬁcance as minerals. They show rather strong relations between chemical composition, synthesis conditions, and the topology of the underlying nets (Table 2). Crystal Structures of Inorganic Oxoacid Salts 41
- 12. g ¼ 1:1. This group of carbonates contains the most abundant CaCO3 minerals (calcite and aragonite) as well as the related magnesite (MgCO3), strontianite (SrCO3), witherite (BaCO3), and cerussite (PbCO3). The calcite and aragonite structure types can be described as oxygen-stuffed NaCl (pcu-b) and anti-NiAs (nia), respectively; M2+ and CO3 2– ions in the aragonite type correspond to As and Ni, respectively [39] (Figs. 3 and 4). There is a strong dependence between the size of M2+ cation and the topological motif: large cations stabilize the aragonite type. Table 2 Underlying nets in carbonates Underlying net Carbonate Correspondencea CO3 coordination type pcu-b (NaCl) MCO3 (M ¼ Mg, Ca, Sr, Ba, Mn, Fe, Co, Ni, Zn, Cd) Normal T6 ; T33 ; T51 nia (NiAs) MCO3 (M ¼ Ca, Sr, Ba, Pb, Eu) Anti Normal (vaterite) T33 T6 bcu (CsCl) CaCO3-HP Normal T44 sqp (SnP) CuCO3 Normal T32 ﬂu (CaF2) Li2CO3 Anti T8 alb (AlB2) Li2CO3-HP Anti T(12) Ni2In (BaF2- HP) M2CO3 (M ¼ Na, K, Rb, Cs) Anti T74 ; T83 ﬁt (MoSi2) Ag2CO3-LT Anti T(10) a Hereafter two kinds of correspondences of M cations and XOn anions to the atoms of a binary compound AyXz (if any) are given in tables: normal or anti if the M cations match the electroposi- tive atoms A or electronegative atoms X, respectively Fig. 3 The NaCl net (Fm3m) and some related nets of oxoacid salts: CaCO3 (calcite) and isostructural MBO3, MNO3 (R3c); BaSeO3 and isostructural PbSO3, MSeO3, KClO3 (P21/m); BaSO4-HT and isostructural MSO4, MClO4 (F43m). Hereafter by default an M atom is placed in the center of the net fragment for any oxoacid salt. Only one representative of each isostructural series is shown 42 V.A. Blatov
- 13. Thus, MgCO3 exists only in the calcite form; for CaCO3 this form is stable at ambient conditions, while MCO3 (M ¼ Sr, Ba, Pb) crystallize in the aragonite type. This tendency is kept for carbonates of d- and f-metals: MCO3 (M ¼ Mn, Fe, Co, Ni, Zn) belong to the calcite type, while EuCO3 has the aragonite-like structure. Calcite-like disordered high-temperature phases are known for SrCO3 and BaCO3 but they are not quenchable [40]. High-pressure phases of CaCO3 (post-aragonite [41]) and BaCO3 [42] have topologically denser 8,8-coordinated CsCl (bcu) and a novel binodal 9,9-coordinated underlying net, respectively. One more metastable phase of CaCO3, the mineral vaterite [43], represents an antitype to aragonite, i.e., M2+ and CO3 2– ions are topologically equivalent to Ni and As atoms in the NiAs- like underlying net. The differences in topologies of the calcite and aragonite underlying nets are reﬂected by different coordination types of carbonate ions: T6 and T33 , respectively (Fig. 5). In both cases, the carbonate ion is connected to six M cations but forms different numbers of M–O bonds: 6 and 9, respectively. As a result, the coordina- tion numbers of cations are larger in the latter case that conforms to large sizes of the cations in the aragonite type. Since the oxoanion has very ﬂexible coordination, it can ﬁt any coordination numbers of cations. An example is the crystal structure of CuCO3, where Cu atoms have CN ¼ 7 but the resulting topology is 5-coordinated Fig. 4 The NiAs net (P63/ mmc) and some related structures of oxoacid salts. Anti-NiAs: CaCO3 (aragonite) and isostructural MCO3, MBO3 (Pnma); normal NiAs: MgSeO3 andisostructural MSeO3, NaIO3 (Pnma); FeSO4 and isostruc- tural MPO4, MSO4, MSeO4 (Cmcm) Crystal Structures of Inorganic Oxoacid Salts 43
- 14. sqp (SnP) net; both Cu and carbonate ions are topologically equivalent in the underlying net. g ¼ 2:1. The thermal polymorphism gives three phases for M2CO3 (M ¼ Na, K, Rb, Cs) with a great variety in space-group symmetries [44, 45] (Table 3). Strictly speaking, these structures cannot be considered as oxygen-stuffed: owing to the large g ratio and large size of the alkali atoms, not all cations are shielded by the oxygens. This leads to abnormal coordination numbers of some alkali atoms and to an essential distortion of their environment. As a result, in all phases there is a large room around the abnormally coordinated alkali atoms; different size of this room gives rise to the structural differences of the polymorphs. However, all these phases can be described in terms of the same underlying net of the Ni2In structure type (Fig. 6), a net of great importance for this stoichiometric g ratio (see [7] and more examples below). For the ionic model, it is important that there is a binary ionic compound, the high-pressure phase of BaF2, which has the same topological motif [46]. Thus, all varieties of these polymorphs are caused by different distortions of the same cation array. The Li2CO3 polymorphs show the typical trend for baric polymorphism: the under- lying net becomes topologically denser in the high-pressure phase. Thus, at ambient conditions the cation array Li2C follows the anti-ﬂuorite (Li2O) 4,8-coordinated motif, but above 10 GPa it transforms to the 5,10-coordinated AlB2-like net. Fig. 5 Most typical coordination types of triangular and trigonal- pyramidal oxoanions Table 3 Space-group symmetries for M2CO3 polymorphs M atom a-phase b-phase g-phase Na P63/mmc C2/m C2/m K P63/mmc C2/c P21/c Rb P63/mmc Pnma P21/c Cs P63/mmc Pnma P21/c 44 V.A. Blatov
- 15. The low-temperature phase of Ag2CO3 also has the 5,10-coordinated underlying net, but of the MoSi2 structure type. 3.1.2 Orthoborates g ¼ 1:1. This is the most numerous group of orthoborates that is topologically closely related to carbonates. Since all these orthoborates are obtained at a high temperature and/or pressure, it is not easy to determine which phase is the most stable at ambient conditions [47]. However, the general trend is similar to carbo- nates: smaller M3+ cations provide the pcu-b cation array (Fig. 3), while larger rare- earth M3+ cations give rise to a nia aragonite-like underlying net (Fig. 4; Table 4). Fig. 6 The Ni2In (BaF2-HP, Pnma) net and some related structures of oxoacid salts: Na2CO3 (C2/m); b-Ca2SiO4 (larnite) and isostructural M2SiO4, Sr2GeO4 (P21/n); Na2SO4 and isostructural M2SO4 (Cmcm) Table 4 Underlying nets in orthoborates Underlying net Orthoborate Correspondence BO3 coordination type pcu-b (NaCl) MBO3 (M ¼ Al, Ti, V, Cr, Fe, Sc, In, Bi, La, Ce, Nd, Dy, Sm, Eu, Yb, Lu) Normal T6 ; T33 ; T42 nia (NiAs) MBO3 (M ¼ La, Ce, Nd) Anti T33 cor (a-Al2O3) M3(BO3)2 (M ¼ Ca, Sr, Hg, Eu) Anti T6 K2Te3 M3(BO3)2 (M ¼ Mg, Mn, Ni, Cd) Anti T71 gfy (UCl3) Tl3BO3 Anti T9 sqc908 Ag3BO3 T(12) Crystal Structures of Inorganic Oxoacid Salts 45
- 16. g ¼ 3:2. The orthoborates of the Ca3(BO3)2 family can be considered as based on a distorted anti-corundum (cor) motif M3B2 if one takes into account the four strongest M–O bonds out of eight oxygens surrounding the M2+ cation (Fig. 7) [48]. The four remaining M–O contacts give rise to additional connections M–B in the cation array and to a new 6,9-coordinated underlying net derived from cor. The series M3(BO3)2 (M ¼ Mg, Mn, Ni, Cd) with octahedrally coordinated M atoms is related to the K2Te3 crystal structure [49] if one ignores Te–Te bonds (Fig. 8). The a, b-Zn3(BO3)2 polymorphs [50], being unique structure types, are topologically close to the cor net since their topological indices are similar (Table 5). One can conclude that the differences are caused by the appearance of eight-cycles in the underlying nets of the polymorphs compared to the cor net. g ¼ 3:1. These cation-rich structures of M3BO3 compounds are also tend to have antitypes as underlying nets; thus, the cation array Tl3B in Tl3BO3 have the topology of 3,9-coordinated UCl3 net (Fig. 9). The Ag3B arrays in two Ag3BO3 phases (obtained at ambient and high pressure) are the ﬁrst examples of 4,12- coordinated epinet sqc908. 3.1.3 Nitrates g ¼ 1:1. At ambient conditions the MNO3 nitrates also show a strong dependence of the underlying net topology on the size of the M+ cation. Like carbonates Fig. 7 The corundum (a- Al2O3) net (R3c) and some related structures of oxoacid salts. Anti-Corundum: Hg3(BO3)2 and isostructural M3(BO3)2 (R3c); normal corundum: Al2(SO4)3 and isostructural M2(SO4)3 (R3) Fig. 8 Topological resemblance between K2Te3 and Mg3(BO3)2 crystal structures 46 V.A. Blatov
- 17. and orthoborates, small cations (Li and Na) provide the pcu-b motif (Fig. 3), while a-KNO3 possesses anti-NiAs (aragonite) underlying topology (Fig. 4; Table 6). In contrast to other compounds with triangular anions, nitrates containing the largest M+ cations (Rb, Cs, Tl) follow the denser 8,8-coordinated CsCl motif that was elucidated in [51]. High-pressure phases have the same (RbNO3-V, CsNO3-III, IV) or denser (KNO3-IV; 7,7-coordinated FeB; Fig. 10) underlying nets compared to phases at ambient conditions. In the former case, the high pressure gives rise to increase in the coordination of anions (from T8 , T71 to T62 , T44 for RbNO3 or CsNO3). The trend is reversed for the high-temperature phase KNO3-III that has Table 5 Topological indices in the underlying nets of a, b-Zn3(BO3)2 polymorphs and some related binary compoundsa Compound Net point symbol Coordination sequence a-Al2O3 {46 .69 }2{43 .63 }3 Al: 6 13 39 46 105 O: 4 16 26 66 70 Rh2O3-HP {45 .69 .8}2{42 .64 }2{43 .63 } Rh: 6 14 42 50 114 O: 4 16–17 28 70–72 76 a-Zn3(BO3)2 {45 .68 .82 }{46 .68 .8}{43 .63 }{44 .62 }2 B(1–4): 6 12–13 37–41 45–49 107–111 Zn(1–6): 4 16–17 25–27 66–69 71–76 b-Zn3(BO3)2 {45 .69 .8}2{42 .64 }{44 .62 }2 B(1–2): 6 13 40 48 111–112 Zn(1–3): 4 16–18 26–27 65–74 74–75 a The indices of metal atoms and the corresponding orthoborate anions are bold; the ranges of terms of the coordination sequences are given for crystallographically nonequivalent atoms Fig. 9 Topological resemblance between UCl3 and Tl3BO3 crystal structures Table 6 Underlying nets in nitrates Underlying net Nitrate Correspondence NO3 coordination type pcu-b (NaCl) MNO3 (M ¼ Li, Na, K, Ag) Normal T6 ; T33 nia (NiAs) a-KNO3 Anti T33 FeB KNO3-IV Anti T34 bcu (CsCl) MNO3 (M ¼ Rb, Cs, Tl) Normal T44 ; T62 ; T71 ; T8 pyr (FeS2) M(NO3)2 (M ¼ Ca, Sr, Ba, Mn, Co, Ni, Cd) Normal T3 ; T21 ; T03 mog (SiO2, moganite) b-Cu(NO3)2 Normal B2 Crystal Structures of Inorganic Oxoacid Salts 47
- 18. topologically less dense underlying net (pcu-b, topological density TD10 ¼ 1,561) than a-KNO3 (nia, TD10 ¼ 1,748). g ¼ 1:2. Almost all nitrates M(NO3)2 investigated by X-rays have the same pyrite-like (pyr) 3,6-coordinated underlying net (Fig. 11); however, the space- group symmetries vary from orthorhombic (Pca21, M ¼ Cd) to rhombohedral (R3, M ¼ Co) and cubic (Pa3, M ¼ Ca, Sr, Ba, Mn, Ni); the highest symmetry coincides with the maximal-symmetry embedding of the pyr net. The coordination numbers of the M atoms also change from 6 (M ¼ Mn, Co, Ni) to 7 (M ¼ Cd) and 12 (M ¼ Ca, Sr, Ba), which results in the corresponding change in coordination type of the nitrate groups: from T3 for CN ¼ 6 to T03 for CN ¼ 12. A special (square) coordination of copper atoms in b-Cu(NO3)2 gives rise to the moganite (mog) motif that is nontypical for cation arrays. 3.2 Oxoacid Salts with Trigonal-Pyramidal Anions This group of ionic compounds is characterized by an asymmetric environment of anions owing to stereochemically active lone electron pair (E-pair). This distortion, being rather strong, often does not allow one to recognize the topological motif of the underlying net just with a visual analysis of the crystal structure. Indeed, the number of correspondences to binary compounds is less compared to the oxoacid Fig. 11 The pyrite-like net (Pa3, S–S contacts are ignored) and some related structures of oxoacid salts: Ca (NO3)2 and isostructural M (NO3)2 (Pa3); a-Sn(SeO3)2 Fig. 10 The FeB net (B–B contacts are ignored) and some related structures of oxoacid salts. Anti-FeB: KNO3-IV; normal FeB: BaSO4 (barite) and isostructural MSO4, BaSeO4, MClO4, and MBrO4 48 V.A. Blatov
- 19. salts considered in the previous part; however, the periodic-graph approach reveals non-strict resemblances in many cases [17]. 3.2.1 Sulﬁtes, Selenites, and Tellurites Sulﬁtes, selenites, and tellurites present some examples of nontrivial topological relationships. According to [17], the b and g phases of HgSeO3 are the ﬁrst example of formally isostructural compounds that have similar geometrical parameters (space group and unit cell dimensions) but different topologies, and hence are related to different topological types. Indeed, both phases belong to the same space group (P21/c) with very close unit cell volumes (309.5 and 306.2 A˚ 3 ) and equal coordination numbers of corresponding atoms. This allowed the author [52] to put them into the same structure type. However, the coordination sequences for b- and g-HgSeO3 differ even in the second coordination shell: in b-HgSeO3 each SeO3 2– anion is bonded to 6 Hg atoms via oxygens, while for g-HgSeO3 the number of Hg atoms in the second coordination shell is 5; the same concerns the numbers of Se atoms in the second coordination shell of Hg atoms. As a result, the underlying nets in these polymorphs have the topologies of 6-coordinated uninodal and 5,5- coordinated binodal nets, derived in [23, 37] from 7-coordinated sev and 6,6- coordinated nia nets, respectively (Table 7). At the same time, the quasi-binary representation allows one to discover similarities between geometrically and topo- logically nonequivalent crystal structures. According to [17], there are three such cases: between Na2SO3, K2SO3, K2TeO3, and Cs2TeO3; between two phases of PbSO3, PbSeO3, and BaSeO3; between CdSO3-II, CdSeO3, and b-MnSO3. In fact, the similarity of topological types in the quasi-binary representation means a topological equivalence of cation arrays or packings of cations and structureless anions. In particular, when comparing the underlying nets, the different coordina- tion types of anions are ignored in Na2SO3 (T901 ) and K2SO3 (T631 ); only the total Table 7 Underlying nets in sulﬁtes and selenites Underlying net Sulﬁte/selenite Correspondence LO3 coordination type pcu-b (NaCl) PbSO3, MSeO3 (M ¼ Sr, Ba, Pb) Normal T33 nia (NiAs) MSeO3 (M ¼ Mg, Mn, Co, Ni, Cu, Zn, Cd, Hg) Normal T6 sev-6-C2/m b-HgSeO3 T51 HIYXUJ CaSeO3 T51 nia-5,5-P21/c CdSO3, g-HgSeO3 T32 bnn (BN) MSeO3 (M ¼ Cu, Zn) Normal T5 Ni2Al Na2SO3 T901 NASTEH M2(SeO3)3 (M ¼ Bi, Er) T31 , T22 stp Sc2(SeO3)3 T4 rtl (TiO2, rutile) M(SeO3)2 (M ¼ Ti, Mn, Sn, Pb) Normal T3 pyr (FeS2) a-Sn(SeO3)2 Normal T3 Crystal Structures of Inorganic Oxoacid Salts 49
- 20. number of coordinated cations (9 þ 0 þ 1 ¼ 6 þ 3 þ 1) is important for the comparison. g ¼ 1:1. The topological types pcu-b and nia play the key role in the cation arrays of selenites MSeO3; however, the dependence on the size of the M2+ cation is inverted compared to the oxoacid salts with triangular anions: large cations provide the pcu-b motif with the T33 coordination type of the anions (Fig. 3), while smaller cations facilitate the formation of the NiAs (nia) array of vaterite type (not anti- NiAs as for most structures considered in Sect. 3.1). Note that the NiAs-like selenites (Fig. 4) are described as distorted perovskite-like structures [53]; these descriptions, however, do not elucidate the relations to other MSeO3 structure types. The coordination types of the LO3 2À anions (T33 and T6 ) correlate with the size of the M2+ cations. It seems reasonable to correlate the inversion with the E-pair. However, the mechanism of this effect remains unexplained so far. This effect gives rise to the appearance of other 6-coordinated underlying nets (sev-6-C2/m and HIYXUJ) that are unique for this group of compounds. sev- 6-C2/m was generated ab initio [23] and has not been found in crystal structures so far. The HIYXUJ underlying topology was revealed quite recently in the lead- organic compound (m6-3,4-dihydro-3-thioxo-1,2,4-triazin-5(2H)-onate)Pb(II) [54] (CSD Reference code HIYXUJ). Both topological types can be considered as intermediate between pcu-b and nia because the topological indices of sev-6-C2/ m and HIYXUJ lie between those of pcu-b and nia (Table 1). The same concerns the pair of 5-coordinated underlying nets bnn and nia-5,5-P21/c; the latter one can be considered as a topological distortion of bnn that has a higher symmetry. g ¼ 2:1. The relations between the cation array Na2S in Na2SO3 and the Ni2Al structure type are discussed in detail in this volume [55]. g ¼ 2:3. The topological types of the underlying nets in M2(LO3)3 are prede- termined by pyramidal (c1 -tetrahedral) form of the coordination ﬁgures of the cations with the stereochemically active E-pair. The corundum motif (cor) is not preferred in this case since the tetrahedral coordination of the 4-coordinated atom in cor does not ﬁt the c1 -tetrahedral form [56]. Therefore, two other 4,6-coordinated nets, stp and NASTEH, appear; they contain square-planar coordination ﬁgures in the most symmetrical embedding (Fig. 12). Both of them were revealed only in metal-organic compounds [57]; stp is quite common (16 examples), NASTEH was found only in (ethane-1,2-diammonium)((m6-ethylenediphosphonato)2Zn3) [58] (CSD Reference code NASTEH). g ¼ 1:2. Two well-known topological types of AB2 ionic compounds, rutile (rtl) and pyrite (pyr), lie in the base of the M(SeO3)2 compounds (Figs. 11 and 13; Fig. 12 Topological resemblance between the stp net (P6/mmm) and Sc2(SeO3)3 50 V.A. Blatov
- 21. Table 7); they emerge in a and b modiﬁcations of Sn(SeO3)2, respectively. The pyrite cation array was also revealed for the M(NO3)2 compounds (Fig. 11; Table 6); the relation between b-Sn(SeO3)2 and M(NO3)2 was reported in [59]. 3.2.2 Chlorates, Bromates, and Iodates The relations of chlorates, bromates, and iodates to binodal nets are quite similar to sulﬁtes and selenites owing to the like geometry and coordination capability of their oxoanions; the differences are mainly caused by a smaller charge of the chlorate-, bromate, or iodate oxoanions compared to sulﬁte or selenite ones and, hence, other possible g ratios (Table 8). g ¼ 1:1. The general trend in the cation array topology follows the features described in the previous part. Large alkali cations promote the pcu-b underlying net, while smaller ones tend to form the NiAs-like underlying net. In both cases, the underlying nets are geometrically distorted in comparison with the ideal pcu-b and Fig. 13 The TiO2 (rutile) net (P42/mnm) and some related structures of oxoacid salts: Ti(SeO3)2; a-Cu(IO3)2 and isotypic M(IO3)2 (P21) Table 8 Underlying nets in chlorates, bromates, and iodates Underlying net Chlorate/bromate/iodate Correspondence LO3 coordination type pcu-b (NaCl) MClO3; MBrO3 (M ¼ Na, K, Rb, Tl); MIO3 (M ¼ K, Tl) Normal T33 , T6 , T42 nia (NiAs) MIO3 (M ¼ Li, Na) Normal T6 crb (CrB4) b-LiIO3 Normal T4 nia-5,5- Pna21 g-LiIO3 T5 FEQWOO NaIO3 T6 Tl2S2 AgClO3 Normal T6 kwh CsBrO3; MIO3 (M ¼ K, Rb) T331 , T61 , T52 bcu-7-Pnnm CsIO3 T331 rtl (TiO2, rutile) M(IO3)2 (M ¼ Mg, Mn, Co, Cu) Normal T3 scu (BaTe2) Ba(LO3)2 (L ¼ Br, I) Normal T31 sqc1964 M(ClO3)2 (M ¼ Sr, Ba, Pb); Ba(BrO3)2 T31 , T4 acs (WC) M(IO3)3 (M ¼ Al, Fe, Ga, In) Normal B2 Crystal Structures of Inorganic Oxoacid Salts 51
- 22. nia nets, thanks to existence of E-pairs (cf. Figs. 3 and 4). Further increase in the size of the M+ cation gives rise to 7-coordinated kwh and bcu-7-Pnnm underlying nets that have not yet been found in binary inorganic compounds. In the high- temperature phases of LiIO3, the coordination of the structure units decreases yielding the 4- and 5-coordinated cation arrays with the crb (boron subnet in CrB4 or the silicon framework in the tectosilicates of the BCT family) and NiAs- related nia-5,5-Pna21 topologies, respectively. A NaIO3 modiﬁcation [60] contains the 6-coordinated underlying net FEQWOO topologically close to nia (Table 1) that was found in [4,40 -bipyridinium](m6-benzene-1,2,4,5-tetracarboxylato)2Pr(III)2 hydrate (CSD Reference code FEQWOO) as well as in 13 other metal-organic frameworks [57]. g ¼ 1:2. There are two main groups of M(LO3)2 compounds: small M2+ cations together with iodine cations form the 3,6-coordinated rutile array as in the corresponding selenites (Table 7), while large alkaline-earth cations and Pb2+ provide topologically denser 4,8-coordinated sqc1964 or scu underlying nets. The scu topological type is related to barium ditelluride (BaTe2) [61] if one ignores Te–Te bonds in the Te2 2– anions (Fig. 14). g ¼ 1:3. A large group of M(IO3)3 iodates contains M3+ cations bridged by iodate anions; the resulting 6-coordinated WC (acs) underlying net does not include the iodine atoms because they transform to edges at the second step of the simpliﬁcation procedure (Fig. 2). Among binary compounds, AgF3 and AuF3 [62] have the same topology as MI3 array in M(IO3)3. According to [63], there is a close relation between MIO3, M(IO3)2, and M(IO3)3 crystal structures: the iodate anions form a pseudo-hexagonal close packing, where M cations occupy all, one half or one third of the octahedral holes, respectively. This reﬂects in more detail the relations between nia, rtl, and acs nets. 3.3 Oxoacid Salts with Tetragonal Anions Tetragonal coordination of a nonmetal cation provides its good shielding; hence, the model of the oxygen-stuffed alloy seems even more valid in this case. The coordination types of XO4 anions are rather diverse (Fig. 15) and provide the topol- ogies with quite different coordination of the nodes. Indeed, many examples of correspondences between this class of oxoacid salts and binary compounds were reported in [4, 7, 16]. Below these results are summarized and updated. Fig. 14 Topological resemblance between the scu (BaTe2) net (P4/mmm, Te–Te contacts are ignored) and the Ba(IO3)2 crystal structure 52 V.A. Blatov
- 23. 3.3.1 Orthosilicates and Orthogermanates g ¼ 1:1. pcu-b and nia topological types, being quite common for most classes of oxoacid salts, have not been found in orthosilicates or orthogermanates; the higher- coordinated underlying nets are more typical for them. The crystal structure of ZrSiO4 (zircon) illustrates a rare case of contradictions in the topology of the underlying net and cation array [16]. O’Keeffe and Hyde [4] found the topological similarity between the ZrSi cation array and the 10-coordinated array of metal atoms in rutile or b-Hg. However, the orthosilicate groups are not condensed in zircon, and the contacts Si–Si existing in the array disappear in the underlying net that has the 6-coordinated uninodal msw topology (Fig. 16a; Table 9). The under- lying net in ThSiO4 (huttonite) is 7-coordinated bcu-7-P21/c (Fig. 16b); it occurs in monoclinic RhSi [64] and in the monazite-type orthophosphates (see below), while the orthosilicates and orthogermanates of the scheelite type contain topologically dense 8-coordinated lsz underlying net (Fig. 16c). g ¼ 2:1. In [4, 7], the olivine (g-Ca2SiO4) structure type was related to PbCl2 (cotunnite) or Ni2In-type cation arrays. In a later review [16], it was shown that the Ca2Si trinodal underlying net in olivine has the same 4,5,9-coordination as the cotunnite net, but starting from the second coordination shell the coordination sequences are different. This is a good illustration of the advantages of the computer approach: in most cases, it is impossible to recognize the differences in outer coordination shells by visual analysis. Instead of olivine, the b-Ca2SiO4 (larnite) structure type has the Ni2In-type underlying net [16] (Fig. 6). Fig. 15 Most typical coordination types of tetrahedral oxoanions Crystal Structures of Inorganic Oxoacid Salts 53
- 24. The oxoanion has its maximal coordination in the spinel-type orthosilicates and orthogermanates; the 6,12-coordinated cation array has the topology of the Laves phase MgCu2, where the contacts Cu–Cu are ignored. The high-pressure chromium and cadmium orthosilicates as well as Hg2GeO4 are characterized by a 5,10- coordinated underlying net of the TiSi2 type [65], where the contacts Si–Si are Fig. 16 Topological resemblances between (a) the msw net (P42/nnm) and ZrSiO4 (zircon); (b) the bcu- 7-P21/c (RhSi) net and ThSiO4 (huttonite); (c) the lsz net (P42/nnm) and ZrSiO4 (scheelite) Table 9 Underlying nets in orthosilicates and orthogermanates Underlying net Orthosilicate/orthogermanate Correspondence XO4 coordination type lsz ZrSiO4; MGeO4 (M ¼ Zr, Hf, Th, U) (scheelite type) Normal K8 bcu-7-P21/c (RhSi) ThSiO4 Normal K52 msw MSiO4 (M ¼ Zr, Hf, Ce, Th) (zircon type) K42 mgc (MgCu2) M2SiO4 (M ¼ Mg, Fe, Co, Ni, Zn, Cd); M2GeO4 (M ¼ Mg, Fe, Co, Ni, Cu) (spinel type) Anti K(12) Ni2In (BaF2-HP) M2SiO4 (M ¼ Ca, Sr, Ba, Eu); Sr2GeO4 Anti K74 , K83 , K92 , K461 , K641 TiSi2 M2SiO4 (M ¼ Cr, Cd); Hg2GeO4 Anti K82 sqc1964 Zn2SiO4-II K8 tph; Th3P4 Bi4(XO4)3 (X ¼ Si, Ge) Anti K8 54 V.A. Blatov
- 25. omitted. Note that this topology differs from other 5,10-coordinated nets (alb and ﬁt) revealed in cation arrays in carbonates (Table 2). One more high-pressure phase, Zn2SiO4-II, has a 4,8-coordinated sqc1964 underlying net that we saw in chlorates (Table 8). g ¼ 4:3. Bi4(SiO4)3 (eulitite) and isostructural Bi4(GeO4)3 have a Th3P4-like cation array [4]. 3.3.2 Orthophosphates and Orthoarsenates g ¼ 1:1. In this group of oxoacid salts, the pcu-b and nia underlying nets are again observed (Table 10). Orthophosphates and orthoarsenates with small trivalent cations belonging to the CrVO4 structure type [66] are based on the nia motif (Fig. 4), while pcu-b is realized only in a high-temperature modiﬁcation of BiPO4 [67]. The underlying nets lsz (scheelite type), bcu-7-P21/c (monazite type), and msw (zircon/xenotime type) found in orthosilicates and orthogermanates (Fig. 15; Table 9) are quite common for orthophosphates and orthoarsenates, which reﬂects well-known relations between these groups of compounds [68]. Orthophosphates and orthoarsenates with tetrahedrally coordinated M3+ cations represent a large group of silica-like structures most of which are microporous Table 10 Underlying nets in orthophosphates and orthoarsenates Underlying net Orthophosphate/orthoarsenate Correspondence XO4 coordination type pcu-b (NaCl) BiPO4-HT Normal K42 nia (NiAs) MPO4 (M ¼ Al, In, Ti, V, Cr, Fe, Tl); MAsO4 (M ¼ Cr, Mn) Normal K6 lsz MPO4 (M ¼ Yb, Lu); MAsO4 (M ¼ Bi, Sm) Normal K8 bcu-7-P21/c (RhSi) MPO4 (M ¼ Bi, La, Ce, Pr, Nd, Sm, Eu, Gd); MAsO4 (M ¼ Bi, La, Ce, Nd) (monazite type) Normal K61 , K52 msw MPO4 (M ¼ Sc, Y, Tb, Dy, Ho, Er, Tm, Lu); MAsO4 (M ¼ Sc, Y, Sm, Eu, Tb, Dy, Ho, Yb, Lu) K42 sma MPO4 (M ¼ La, Ce, Nd) K42 nia-5,5-P21/c FeXO4 (X ¼ P, As) K5 dia-b (ZnS, sphalerite) MPO4 (M ¼ Al, Ga); AlAsO4 Normal K4 qtz (a-HgS) MPO4 (M ¼ Al, Fe, Ga); MAsO4 (M ¼ Al, Ga) Normal K4 lon (ZnS, wurtzite) AlPO4 Normal K4 alw (Rh2O3-HP) Sb2(PO4)3 Normal K4 cor (a-Al2O3) Nb2(PO4)3 Normal K4 XEBHOB M3(PO4)2 (M ¼ Mg, Co, Zn); Zn3(AsO4)2 K61 Cu3Sb Li3XO4 (X ¼ P, As) Normal K(12) ith (Cr3Si) Ag3XO4 (X ¼ P, As) Normal K(12) wzz K3AsO4 K68 Crystal Structures of Inorganic Oxoacid Salts 55
- 26. zeolite-like [69] and can hardly be considered within the cation array model. Three “dense” structure types are “grey-isomorphic” to quartz (qtz), cristobalite, or tridymite [70]; in the quasi-binary representation they correspond to a-HgS, sphal- erite (dia-b), and wurtzite (lon), respectively. The underlying nets of other orthophosphates correspond to the phases metasta- ble at ambient conditions. Hexagonal modiﬁcations of lanthanum, cerium, and neodymium phosphates are based on the 6,6-coordinated sma topology (Fig. 17). FePO4 obtained by the “soft” chemistry method [71] has the nia-5,5-P21/c cation array that was also revealed in sulﬁtes and selenites (Table 7). Alternative descrip- tions of both FeLiPO4 and FePO4, in terms of the extended Zintl–Klemm concept, can be found in this volume [72] g ¼ 2:3. Two orthophosphates with this g ratio have similar, but not equivalent topologies: Nb2(PO4)3 has the topology of the Nasicon framework with the corundum- like underlying net (Fig. 7), while Sb2(PO4)3 adopts the motif of a high-pressure modiﬁcation of Rh2O3 [73] to be topologically close to corundum (Table 5). This is one more example of resemblance between the oxygen-stuffed alloys and high- pressure forms of the corresponding binary compounds (cf. [7]). g ¼ 3:2. Most of the orthophosphates and orthoarsenates of this g ratio have complex polynodal underlying nets with a unique topology; the relations to known topologies of nets are occasional. Thus, the structure type of farringtonite, Mg3(PO4)2, has the trinodal 4,6,7-coordinated underlying net that was found in Mn3(m7-phosphonopropionato)2 (CSD Reference code XEBHOB) [74]. g ¼ 3:1. According to [4], the cation array in Ag3PO4 is similar to the 14,12- coordinated Cr3Si (b-W) crystal structure that reﬂects the spatial arrangement of Ag and P atoms. If one neglects Ag–Ag contacts, a 4,12-coordinated ith underlying net (UH3 structure type [16]) emerges that is a subnet of Cr3Si. Lithium orthophosphate and orthoarsenate contain a Cu3Sb-like cation array [4] that represents a distorted hexagonal close packing where the underlying net with only Cu-Sb (Li-P) contacts is trinodal 4,4,12-coordinated. The recently investigated crystal structure of K3AsO4 [75] is the ﬁrst example of the complex trinodal 4,6,14-coordinated wzz underlying net. 3.3.3 Sulfates and Selenates g ¼ 1:1. The pcu-b and nia underlying nets are quite common for sulfates and selenates (Table 11). Small 6-coordinated M2+ cations promote a nia cation array Fig. 17 Topological resemblance between the sma net (P6222) and the LaPO4 crystal structure 56 V.A. Blatov
- 27. [7] (Fig. 4), while 8-coordinated Ca and Hg provide a pcu-b underlying net (Fig. 3). At ambient conditions, sulfates and selenates with large alkaline-earth cations adopt a 7,7-coordinated FeB-like motif (Fig. 10) and transform to pcu-b only at high temperature. CaSO4 has 7,7-coordinated underlying nets FeB and RhSi (monazite- like) under high pressure [76]. The high-temperature g-CaSO4 is an example of reorganization of the anhydrite cation array (pcu-b) to another 6,6-coordinated net with the sma topology (Fig. 17). Note that g-CaSO4 is obtained by a “soft chemis- try” method (heating CaSO4Á0.5H2O, cf. the method of obtaining orthophosphates with the sma cation array; Table 10). 4-coordinated Be2+ , Zn2+ , and Pd2+ cations together with 4-coordinated S or Se cations form sphalerite- or PtS-like arrays. The topology is predetermined by the coordination ﬁgures of the M and X cations: tetrahedral coordination ﬁgures give rise to the sphalerite motif while the rect- angle þ tetrahedron combination (PdXO4) results in the similar PtS (cooperite) array (Fig. 18). g ¼ 2:1. Most sulfates and selenates of this type have the 5,6,11-coordinated Ni2In-like cation array [16] (Fig. 6). In [7], caesium sulfate and selenate were related to the cotunnite (PbCl2) structure type. This is an example of discrepancies between geometrical and topological descriptions obviously caused by the close topologies of the PbCl2 and Ni2In crystal structures. At the same time, the cation array in the high-temperature Na2SO4 phase was assigned to the Ni2In type [6] that conﬁrms the conclusion of the periodic-graph approach. At ambient conditions, Table 11 Underlying nets in sulfates and selenates Underlying net Sulfate/selenate Correspondence XO4 coordination type pcu-b (NaCl) MSO4 (M ¼ Ca, Sr, Ba, Cd, Hg); HgSeO4 Normal K42 , K51 , K06 nia (NiAs) MSO4 (M ¼ Mg, Mn, Fe, Co, Ni, Cu, Cd, Zn); MSeO4 (M ¼ Mg, Mn, Co, Ni, Cu) Normal K6 ﬂu (CaF2) Li2SO4 Anti K8 FeB MSO4 (M ¼ Ca, Sr, Ba, Pb, Eu); BaSeO4 Normal K43 , K61 bcu-7-P21/c (RhSi) CaSO4-HP, MSeO4 (M ¼ Sr, Pb) Normal K52 , K61 sma g-CaSO4 K42 dia-b (ZnS, sphalerite) MSO4 (M ¼ Be, Zn) Normal K4 pts (PtS) PdXO4 (X ¼ S, Se) Normal K4 Ni2In (BaF2-HP) M2SO4 (M ¼ Li, Na, K, Rb, Cs, Tl); M2SeO4 (M ¼ K, Cs, Tl) Anti K461 , K47 , K65 , K56 , K911 , K(10)1 TiSi2 M2XO4 (M ¼ Na, Ag; X ¼ S, Se) Anti K82 alw (Rh2O3-HP) M2(SO4)3 (M ¼ Fe, In, Y, Er); M2(SeO4)3 (M ¼ Fe, Sc, Yb) Normal K4 cor (a-Al2O3) M2(SO4)3 (M ¼ Al, Ga, Cr, Fe, In, Sc) Normal K4 PbCl2 (cotunnite) a-Zr(SO4)2 Normal T3 , K4 Crystal Structures of Inorganic Oxoacid Salts 57
- 28. Na2SO4 (thenardite), as well as the Ag2SO4 cation array, adopts the 5,10-coordinated TiSi2-like motif [16]. This means that the reported relations between thenardite and the spinel structure type as well as between other Na2SO4 modiﬁcations and the olivine structure type [6] reﬂect geometrical similarities of the structure types, but do not take into account all their topological features. As was mentioned in Sect. 3.3.1, the olivine structure type is not topologically equal to the Ni2In type, also the TiSi2 underlying net does not coincide with the spinel-like net. This example demonstrates that visual analysis cannot detect some tiny topological differences, although the general (not strict) similarities of the motifs under consid- eration are unquestionable. The reader is referred to two chapters of this volume [55, 72] where the structures are analyzed visually, producing discrepancies with the results exposed here. g ¼ 2:3. Like orthophosphates (Table 10), some sulfates and selenates of this g ratio adopt two topological types of binary compounds: alw and cor. The corundum- like cation array typical for this g ratio is realized for most sulfates of trivalent d-elements (Fig. 7); however, for large M cations alw is more preferable. g ¼ 1:2. The only representative of this g ratio, a-Zr(SO4)2, is related to cotun- nite (PbCl2) if one ignores two long (3.65A˚ ) Pb–Cl contacts and considers the cotunnite net as 3,4,7-coordinated, not 4,5,9-coordinated. 3.3.4 Perchlorates, Perbromates, and Periodates g ¼ 1:1. There are clear dependences of the underlying net topology on the kind of M+ cation and XO4 – anion (Table 12). For perchlorates, the increase in the M+ cation size in the row Li–Na–K, Rb, Cs gives rise to the sequence nia–pcu-b–FeB at ambient conditions, while the cation arrays in the high-temperature modiﬁcation of MClO4 (M ¼ K, Rb, Cs) decrease their topological density and transform to the pcu- b type. The FeB-like NaClO4 was obtained by chance in the presence of cucurbit[5] uril ions in the mother solution [77]. Perbromates and periodates prefer to have denser Fig. 18 Topological resemblances between (a) ZnS (sphalerite) net (F43m) and ZnSO4; (b) PtS net (P42/ mmc) and PdSO4 58 V.A. Blatov
- 29. cation arrays (in particular, 8,8-coordinated scheelite-like lsz; Fig. 16c) than the corresponding perchlorates. The data of Table 12 agree with the results of Vegas and Jansen [7] as well as with other known relations between perhalogenates and other classes of oxoacid salts with tetrahedral anions (scheelite-like structures [78] as well as NiAs-like orthophosphates and sulfates [79], cf. Tables 9, 10, and 11). g ¼ 1:3. This group is represented only by lanthanide perchlorates that exist in two crystalline forms: at ambient conditions the cation array is of the UCl3 (gfy) type [80] (Fig. 9) for all lanthanides except Lu, and the topologically less dense ReO3-like Tm(ClO4)3 and Yb(ClO4)3 were obtained at a high temperature [80, 81]. In both cases, the perchlorate anion is tridentate but connects to a different number of metal atoms (3 and 2 for T3 and T11 coordination types, respectively) that results in the difference in topological density. 3.4 Uniformity of Cation Arrays in Inorganic Oxoacid Salts The term “eutaxy” as applied to cation arrays means rather ordered, regular arrangement of the cations in the crystal space. In [2, 4], the eutactic placement was treated similarly to a close sphere packing with 12 cations in the vicinity of the given one. However, in the model of cation array the cations should be considered as point charges rather than the rigid bodies touching each other. In this case, the close-packing arrangement could not be a criterion of the “best” placement. In fact, in the most eutactic arrangement the cations should be allocated farthest from each other, i.e., the cation sublattice covers the crystal space most uniformly. The uniformity can be estimated with the formula [82]: G3h i ¼ 1 3 1 Z PZ i¼1 Ð VPðiÞ R2 dVVPðiÞ 1 Z PZ i¼1 VVPðiÞ 5 3 ; Table 12 Underlying nets in perchlorates, perbromates, and periodates Underlying net Perchlorates/perbromates/periodates Correspondence XO4 coordination type pcu-b (NaCl) MClO4 (M ¼ Na, K, Rb, Cs, Tl, Ag) Normal K42 , K06 nia (NiAs) LiClO4 Normal K6 lsz CsBrO4; MIO4 (M ¼ Na, K, Rb, Cs, Tl, Ag) Normal K8 , K62 , K44 FeB MClO4 (M ¼ Na, K, Rb, Cs); MBrO4 (M ¼ K, Tl) Normal K43 nia-5,5-P21/c LiIO4 K5 gfy (UCl3) M(ClO4)3 (M ¼ La, Ce, Pr, Nd, Sm, Eu, Ho, Er, Tm, Yb) Normal T3 ReO3 M(ClO4)3 (M ¼ Tm, Yb, Lu) Normal T11 Crystal Structures of Inorganic Oxoacid Salts 59
- 30. where Z is the number of cations in the asymmetric unit of the array, VVP(i) is the volume of the Voronoi polyhedron of the ith cation, R is the distance between the cation and a point inside its Voronoi polyhedron; G3 is equal to the root-mean- square error of the corresponding space quantizer [83]. The G3 value is computed irrespective of the structure topology; however, the topology of the ion array with a given G3 value can be unambiguously determined from the corresponding packing graph. The least-distorted (i.e., the most uniform) array has the minimum G3; in such an array the cation domains (space regions being most close to the corresponding cations) cover the crystal space most economically. The most uniform placement of points in three-dimensional space is the b.c.c. (bcu-x) lattice with G3 ¼ 0.0785433. . ., while close packings with G3 ¼ 0.07875. . . [83] are less uniform. This means that the b.c.c. lattice with 14 (8 þ 6) neighbors surrounding each cation in the array should also be important for eutactic arrangements. According to [15], the G3 value can be used to determine the structure-forming role of the array: the most uniform array makes the main contribution to the Coulomb energy of the ionic structure. This approach was applied to all kinds of ion arrays in inorganic oxoacid salts My(LO3)z [15, 17]: cation (M), (L), (M + L), anion (O), and mixed cation–anion (M þ O) arrays. It was shown that usually the most uniform array includes all cations (M þ L), and the corresponding packing graph has the bcu-x (rarer fcu) topology. In general, the uniformity of the cation array increases along with the cation charge and size. For instance, in the series of alkaline carbonates M2CO3 the G3 values for the (M) arrays decrease from 0.0876 (M ¼ Li) to 0.0834 (M ¼ Cs) [15]. It was shown [17] that in high-temperature and high-pressure phases the structure-forming cation arrays become more uniform because the ambient factors promote an increase in uniformity and symmetry of the structure-forming array. These results prove the model of cation array but focus the role of the b.c.c. packing along with the close packing motifs. 4 General Regularities in the Cation Arrays The crystal structure data discussed above reveal the following general regularities in the cation arrays perceived as underlying nets of the oxoacid salts. 1. The underlying net usually has rather simple topology corresponding to a well- known topological type. Indeed, of the 569 crystal structures of oxoacid salts considered in this review, only 157 have novel topologies of their cation arrays. The remaining 412 cation arrays belong to 55 topological types of binary compounds or other binodal nets. For a given g ratio there are a few (one or two) preferable (default [31]) underlying nets that frequently occur in nature; the rare nets can be treated as topological distortions of the default nets. The underlying nets can be of three types: (a) quite common (default) for different classes of inorganic compounds (Table 13); (b) typical only for a given class or 60 V.A. Blatov
- 31. closely related compounds, like mgc (MgCu2), this is often caused by an unusual g ratio like 5:3 in Mn3 II Mn2 III (SiO4)3 [84] or 7:6 in Fe3 II Fe4 III (AsO4)6 [85]; (c) occurring occasionally due to special conditions of synthesis (high temperature, pressure, particular experimental methods like “soft chemistry”). All 165 cation arrays with novel topologies belong to types (b) and (c). 2. The overall topology of an underlying net is essentially predetermined by the geometrical forms of coordination ﬁgures of nodes. For example, if the net has square-planar coordination ﬁgures it unlikely corresponds to an oxoacid salt with tetrahedral anions, but can ﬁt a compound with pyramidal anions. The form of the coordination ﬁgure depends on the relative sizes of cations and complex anions; the dependence is similar to that for simple ionic compounds [15]. The coordination capability of the oxoanion predetermines the coordination ﬁgure; the more ﬂexible such capability the larger number of the overall topologies to which the oxoanion can ﬁt (Figs. 5 and 15). 3. The size of cation inﬂuences the topological motif of the cation array; this is evident for the most abundant topological types pcu-b and nia: small or large M cations promote the formation of different underlying nets. Which topological type is realized depends on the nature of the L or X cation. 4. In high-pressure modiﬁcations, the topological density of the underlying net increases, while high-temperature polymorphs have a less dense underlying net than the title compound at ambient conditions. Table 13 Default underlying nets of frequency !8 in 569 crystal structures of inorganic oxoacid salts Underlying net AyXz Coordination number of A/X No. of structures Groups of oxoacid salts g ¼ 1:1 pcu-b (NaCl) 6/6 80 MLO3 (L ¼ B, C, N, S, Se, Cl, Br, I); MXO4 (X ¼ P, S, Se, Cl) nia (NiAs) 6/6 56 MLO3 (L ¼ B, C, N, Se, I); MXO4 (X ¼ P, As, S, Cl) msw (zircon) 6/6 25 MXO4 (X ¼ Si, Ge, P, As) lsz (scheelite) 8/8 22 MXO4 (X ¼ Si, Ge, P, As, Br, I) bcu-7-P21/c (RhSi, monazite) 7/7 17 MXO4 (X ¼ Si, P, As, S, Se) FeB 7/7 15 KNO3; MXO4 (X ¼ S, Se, Cl, Br) dia-b (ZnS, sphalerite) 4/4 9 MXO4 (X ¼ P, As, S) bcu (CsCl) 8/8 8 MLO3 (L ¼ C, N) g ¼ 1:2 (2:1) Ni2In (BaF2-HP) 11/5, 6 24 M2CO3; M2XO4 (X ¼ Si, Ge, S, Se) mgc (MgCu2) 6/12 15 M2XO4 (X ¼ Si, Ge) rtl (TiO2, rutile) 6/3 10 M(LO3)2 (L ¼ Se, I) pyr (FeS2, pyrite) 6/3 9 M(LO3)2 (L ¼ N, Se) g ¼ 2:3 (3:2) alw (Rh2O3-HP) 6/4 10 M2(XO4)3 (X ¼ P, S, Se) cor (a-Al2O3) 6/4 8 M3(BO3)2; M2(SO4)3; Nb2(PO4)3 Crystal Structures of Inorganic Oxoacid Salts 61
- 32. 5. In some cases, the cation array in an oxoacid salt corresponds to the underlying net of a metal-organic compound; no similar inorganic binary compound has been found so far. This could be a challenge to synthetic chemists to obtain such analog. This fact also shows that underlying nets in inorganic and metal-organic compounds have common topological properties. The eutactic distribution of cations in the array is a consequence of their tendency to a uniform arrangement in the crystal space. This trend is inﬂuenced by the following features of the array: 1. The most preferable topological motifs (packing nets) for the cation arrays are b.c.c. and close packings; in most cases, the b.c.c. motif is the most uniform. Hence, the main structure-forming role in the oxoacid salts belongs to cations; the eutactic oxygen arrays are rather rare. 2. Increase in size and charge of the cations results in an increase in the array uniformity. 3. High temperature and pressure favor increase in the uniformity of the structure- forming (most uniform) cation array. 4. Increase in the uniformity changes the topological motif of the cation array: it tends to be b.c.c. The increase in the uniformity of the structure-forming array accompanies decrease in the uniformity of other ion sublattices [17]. These regularities seem to be valid not only for oxygen-stuffed cation arrays but also for ionic compounds containing other anions [86]. 5 Concluding Remarks The periodic-graph approach now is well developed for metal-organic coordination compounds [19] and can give fruitful results when analyzing typical inorganic substances. The main advantages of this approach over visual (even computer- aided) exploration of crystal structures are as follows: (1) its algorithms are formal, strict, and universal, and they are used for any crystal structure according to a common scheme; (2) the topology of an atomic net is unambiguously determined by a set of numerical indices; (3) the concept of the underlying net allows one to easily classify crystal structures of complex compounds by reducing them to simpler topologies and using computer databases of reference nets; (4) the concept of packing net formalizes the analysis of cation arrays: they are classiﬁed with the topological indices; and (5) the topological software provides fast processing hundreds and thousands of structures in a reasonable time. The recent results of the topological analysis of cation arrays in the inorganic crystal structures described in this review underline the importance of the model of cation array and show that the number of preferable (“default”) topological motifs is rather small. We have good cause to believe that this fact, as well as the developed software, opens the door to a comprehensive taxonomy of inorganic 62 V.A. Blatov
- 33. ionic compounds. The experimental data on the high stability of particular topolog- ical motifs of cation arrays could be a reliable background for ab initio modeling of new inorganic substances and materials. Acknowledgments This work was partially supported by a Cariplo Fellowship issued by Cariplo Foundation Landau Network, Centro Volta (Como, Italy). The author thanks Prof. D.M. Proserpio for fruitful discussions of the periodic-graph problems and Dr. A. Vegas for thorough reading of the manuscript and useful comments. References 1. Lebedev VI (1972) Foundations of new crystal chemistry. Int Geol Rev 14:543–547 2. O’Keeffe M (1977) On the arrangement of ions in crystals. Acta Crystallogr A 33:924–927 3. O’Keeffe M, Hyde BG (1981) The role of non-bonded forces in crystals. In: O’Keeffe M, Navrotsky A (eds) Structure and bonding in crystals. Wiley, New York 4. O’Keeffe M, Hyde BG (1985) An alternative approach to non-molecular crystal structures. With emphasis on the arrangements of cations. Struct Bond 61:77–144 5. Borisov SV (2000) Geometrical laws in inorganic chemistry. Crystallogr Rep 45:709–713 6. Vegas A, Grzechnik A, Syassen K (2001) Reversible phase transitions in Na2S under pressure: a comparison with the cation array in Na2SO4. Acta Crystallogr B 57:151–156 7. Vegas A, Jansen M (2002) Structural relationships between cations and alloys; an equivalence between oxidation and pressure. Acta Crystallogr B 58:38–51 8. Krivovichev SV (2009) Structural crystallography of inorganic oxysalts. Oxford University Press Inc, New York 9. Santamarı´a-Pe´rez D, Vegas A (2003) The Zintl-Klemm concept applied to cations in oxides. I. The structures of ternary aluminates. Acta Crystallogr B 59:305–323 10. Santamarı´a-Pe´rez D, Vegas A, Liebau F (2005) The Zintl–Klemm concept applied to cations in oxides. II. The structures of silicates. Struct Bond 118:121–177 11. Vegas A, Garcı´a-Baonza V (2007) Pseudoatoms and preferred skeletons in crystals. Acta Crystallogr B 63:339–345 12. Vegas A, Martin RL, Bevan DJM (2009) Compounds with a ‘stuffed’ anti-bixbyite-type structure, analysed in terms of the Zintl–Klemm and coordination-defect concepts. Acta Crystallogr B 65:11–21 13. Zintl E (1939) Intermetallische Verbindungen. Angew Chem 52:1–6 14. Hewaidy IF, Busmann E, Klemm W (1964) Die Struktur der AB-Verbindungen der schweren Alkalimetalle mit Zinn und Blei. Z Anorg Allg Chem 328:283–293 15. Blatov VA, Zakutkin YA (2002) Comparative topological analysis of simple anhydrous borates, carbonates and nitrates. Z Kristallogr 217:464–473 16. Ilyushin GD, Blatov VA, Zakutkin YA (2004) Orthotetrahedral crystal structures My(TO4)z (T ¼ Si, Ge, P, As, S, Se, Cl, Br, I): geometrical-topological analysis, quasi-binary represen- tation, and comparison with the AyXz compounds by the method of coordination sequences. Z Kristallogr 219:468–478 17. Blatov VA, Peskov MV (2006) A comparative crystallochemical analysis of binary com- pounds and simple anhydrous salts containing pyramidal anions LO3 (L ¼ S, Se, Te, Cl, Br, I). Acta Crystallogr B 62:457–466 18. Blatov VA (2006) Multipurpose crystallochemical analysis with the program package TOPOS. IUCr CompComm Newsletter 7:4–38 19. Blatov VA, Carlucci L, Ciani G, Proserpio DM (2004) Interpenetrating metal-organic and inorganic 3D networks: a computer-aided systematic investigation. Part I. Analysis of the Cambridge structural database. CrystEngComm 6:377–395 Crystal Structures of Inorganic Oxoacid Salts 63
- 34. 20. Francl M (2009) Stretching topology. Nat Chem 1:334–335 21. Delgado-Friedrichs O, O’Keeffe M (2005) Crystal nets as graphs: terminology and deﬁni- tions. J Solid State Chem 178:2480–2485 22. Blatov VA (2006) A method for hierarchical comparative analysis of crystal structures. Acta Crystallogr A 62:356–364 23. Blatov VA (2007) Topological relations between three-dimensional periodic nets. I. Uninodal nets. Acta Crystallogr A 63:329–343 24. Chung SJ, Hahn T, Klee WE (1984) Nomenclature and generation of three-periodic nets: the vector method. Acta Crystallogr A 40:42–50 25. Klee WE (2004) Crystallographic nets and their quotient graphs. Cryst Res Technol 39:959–968 26. Eon J-G (2005) Graph-theoretical characterization of periodicity in crystallographic nets and other inﬁnite graphs. Acta Crystallogr A 61:501–511 27. Thimm G (2009) Crystal topologies - the achievable and inevitable symmetries. Acta Crystal- logr A 65:213–226 28. Delgado-Friedrichs O, O’Keeffe M (2003) Identiﬁcation of and symmetry computation for crystal nets. Acta Crystallogr A 59:351–360 29. Blatov VA, O’Keeffe M, Proserpio DM (2010) Vertex-, face-, point-, Schl€aﬂi-, and Delaney- symbols in nets, polyhedra and tilings: recommended terminology. CrystEngComm 12: 44–48 30. Baburin IA, Blatov VA (2007) Three-dimensional hydrogen-bonded frameworks in organic crystals: a topological study. Acta Crystallogr B 63:791–802 31. Ockwig NW, Delgado-Friedrichs O, O’Keeffe M, Yaghi OM (2005) Reticular chemistry: occurrence and taxonomy of nets and grammar for the design of frameworks. Acc Chem Res 38:176–182 32. Blatov VA (2001) Topological analysis of ionic packings in crystal structures of inorganic sulﬁdes: the method of coordination sequences. Z Kristallogr 216:165–171 33. Wells AF (1954) The geometrical basis of crystal chemistry. Part 1. Acta Crystallogr 7:535–544 34. Delgado-Friedrichs O, O’Keeffe M, Yaghi OM (2007) Taxonomy of periodic nets and the design of materials. Phys Chem Chem Phys 9:1035–1043 35. O’Keeffe M, Peskov MA, Ramsden SJ, Yaghi OM (2008) The reticular chemistry structure resource (RCSR) database of, and symbols for, crystal nets. Acc Chem Res 41:1782–1789 36. Hyde ST, Delgado Friedrichs O, Ramsden SJ, Robins V (2006) Towards enumeration of crystalline frameworks: the 2D hyperbolic approach. Solid State Sci 8:740–752 37. Blatov VA, Proserpio DM (2009) Topological relations between three-periodic nets. II. Binodal nets. Acta Crystallogr A 65:202–212 38. Serezhkin VN (2007) Some features of stereochemistry of U(VI). In: Krivovichev SV, Burns PC, Tananaev IG (eds) Structural chemistry of inorganic actinide compounds, 1st edn. Elsevier, Amsterdam 39. Bevan DJM, Rossmanith E, Mylrea DK et al (2002) On the structure of aragonite – Lawrence Bragg revisited. Acta Crystallogr B 58:448–456 40. Antao SM, Hassan I (2007) BaCO3: high-temperature crystal structures and the Pmcn ! R3m phase transition at 811 C. Phys Chem Miner 34:573–580 41. Ono S, Kikegawa T, Ohishi Y, Tsuchiya J (2005) Post-aragonite phase transformation in CaCO3 at 40 GPa. Am Mineral 90:667–671 42. Holl CM, Smyth JR, Laustsen HMS et al (2000) Compression of witherite to 8 GPa and the crystal structure of BaCO3II. Phys Chem Miner 27:467–473 43. Wang J, Becker U (2009) Structure and carbonate orientation of vaterite (CaCO3). Am Mineral 94:380–386 44. Dinnebier RE, Vensky S, Jansen M, Hanson JC (2005) Crystal structures and topological aspects of the high-temperature phases and decomposition products of the alkali-metal oxalates M2[C2O4] (M ¼ K, Rb, Cs). Chem Eur J 11:1119–1129 64 V.A. Blatov
- 35. 45. Swainson IP, Dove MT, Harris MJ (1995) Neutron powder diffraction study of the ferroelastic phase transitionand lattice melting in sodium carbonate, Na2CO3. J Phys Condens Matter 7: 4395–4417 46. Leger JM, Haines J, Atouf A et al (1995) High-pressure x-ray- and neutron-diffraction studies of BaF2: An example of a coordination number of 11 in AX2 compounds. Phys Rev B 52: 13247–13256 47. Goubin F, Montardi Y, Deniard P et al (2004) Optical properties of CeBO3 and CeB3O6 compounds: ﬁrst-principles calculations and experimental results. J Solid State Chem 177: 89–100 48. Vegas A (1985) New description of the Ca3(BO3)2 structure. Acta Crystallogr C 41: 1689–1690 49. Seifert-Lorenz K, Hafner J (2002) Crystalline intermetallic compounds in the K-Te system: the Zintl-Klemm principle revisited. Phys Rev B 66:094105-1-094105-15 50. Chen X, Xue H, Chang X et al (2006) Syntheses and crystal structures of the a- and b-forms of zincorthoborate, Zn3B2O6. J Alloys Compd 425:96–100 51. Sastry PUM, Rajagopal H, Sequeira A (1994) Thallous nitrate(III); a single-crystal neutron study. Acta Crystallogr C 50:1854–1857 52. Weil M (2002) Preparation and crystal structures of two new modiﬁcations of mercury(II) selenite(IV), HgSeO3, and the mixed-valent mercury(II) selenite(IV) selenide(-II), (HgSeO3)3HgSe. Solid State Sci 4:1153–1162 53. Koskenlinna M, Valkonen J (1995) Mercury(II) selenite. Acta Crystallogr C 51:1040–1042 54. Casas JS, Castellano EE, Ellena J et al (2008) Lead(II)-induced formation and coordination of 3, 4-dihydro-3-thioxo-1, 2, 4-triazin-5(2H)-one. Inorg Chem Commun 11:423–426 55. Vegas A (2011) Missing links in two structural journeys: From stuffed-wurtzite to MoSi2. From stuffed-tridymite to Ba2SnO4. Struct Bond 56. Wontcheu J, Schleid T (2003) Sc2Se3O9: Scandium(III) oxoselenate(IV) according to Sc2(SeO3)3 with a hexagonal “lone-pair” channel structure. Z Anorg Allg Chem 629:1463–1465 57. Alexandrov EV, Blatov VA, Kochetkov AV, Proserpio DM (2010) Underlying nets in coordination frameworks: topology, taxonomy, prediction, and computer-aided analysis of the Cambridge Structural Database. CrystEngComm, submitted 58. Natarajan S (2004) Synthesis and structure of a three-dimensional organically templated zinc ethylenediphosphonate, [NH3(CH2)2NH3][Zn3{O3P(CH2)2}4]. Z Anorg Allg Chem 630: 291–295 59. Steinhauser G, Luef C, Wildner M, Giester G (2006) Syntheses and crystal structures of Pb(SeO3)2 and two modiﬁcations of Sn(SeO3)2. J Alloys Compd 419:45–49 60. Sorokina NI, Ilyukhin VV, Pakhomov VI, Belov NV (1979) About the crystal structure of sodium iodate. Dokl Akad Nauk SSSR 249:613–616 61. Li J, Guo H-Y, Carey JR et al (1994) Synthesis and crystal stucture of a new alkaline-earth metal chalcogenide: barium ditelluride. Mater Res Bull 29:1041–1048 62. Zemva B, Lutar K, Jesih A et al (1991) Silver triﬂuoride: preparation, crystal structure, some properties, and comparison with AuF3. J Am Chem Soc 113:4192–4198 63. Phanon D, Mosset A, Gautier-Luneau I (2007) New materials for infrared non linear optics. Syntheses, structural characterisations, second harmonic generation and optical transparency of M(IO3)3 metallic iodates. J Mater Chem 17:1123–1130 64. Schellenberg L, Jorda JL, Muller J (1985) The rhodium-silicon phase diagram. J Less Common Met 109:261–274 65. Tanaka K, Nawata K, Inui H, Yamaguchi M, Koiwa M (2001) Reﬁnement of crystallographic parameters in refractory metaldisilicides. Mater Res Soc Symp Proc 646:N4.3.1–N4.3.5 66. Glaum R, Reehuis M, Stuesser N et al (1996) Neutron diffraction study of the nuclear and magnetic structure of the CrVO4 type phosphates TiPO4 and VPO4. J Solid State Chem 126:15–21 67. Masse R, Durif A (1985) Etude structurale de la forme haute temperature du monophosphate debismuth BiPO4. Compt Rend Heb Seances Acad Sci 300:849–851 Crystal Structures of Inorganic Oxoacid Salts 65
- 36. 68. Zhang FX, Lang M, Ewing RC et al (2008) Pressure-induced zircon-type to scheelite-type phase transitions on YbPO4 and LuPO4. J Solid State Chem 181:2633–2638 69. Cao G, Afeworki M, Kennedy GJ (2007) Crystal structure of an aluminophosphate EMM-8: a multi-technique approach. Acta Crystallogr B 63:56–62 70. Graetsch H (2000) Two Forms of aluminium phosphate tridymite from X-ray powder data. Acta Crystallogr C 56:401–403 71. Song Y, Zavalii PY, Suzuki M, Whittingham MS (2002) New iron(III) phosphate phases: crystal structure and electrochemical and magnetic properties. Inorg Chem 41:5778–5786 72. Vegas A (2011) LiFePO4: Dissection of a crystal structure. The parts and the whole. Struct Bond. doi:10.1007/430_2010_35 73. Shannon RD, Prewitt CT (1970) Synthesis and structure of a new high pressure form of Rh2O3. J Solid State Chem 2:134–136 74. Stock N, Frey SA, Stucky GD, Cheetham AK (2000) Synthesis and characterization of two manganese phosphonocarboxylates: Mn3(O3PCH2COO)2 and Mn3(O3PCH2CH2COO)2. J Chem Soc Dalton Trans 4292–4296 75. Emmerling F, Idilbi M, Roehr C (2002) Neue Oxopnictate A3 I MV O4: Darstellung und Kristallstruktur von A3AsO4 (A ¼ K, Rb, Cs) und K3BiO4. Z Naturforsch B Chem Sci 57:599–604 76. Crichton WA, Parise JB, Antao SM, Grzechnik A (2005) Evidence for monazite-, barite-, and AgMnO4 (distorted barite)-type structures of CaSO4 at high pressure and temperature. Am Mineral 90:22–27 77. Zhang G-L, Li Y-T, Wu ZY, Song Y-L (2006) Sodium perchlorate in the space group Pnma. Acta Crystallogr E 62:i150–i151 78. Kalman A, Cruickshank DWJ (1970) Reﬁnement of the structure of NaIO4. Acta Crystallogr B 26:1782–1785 79. Wickleder MS (2003) Crystal structure of LiClO4. Z Anorg Allg Chem 629:1466–1468 80. Pascal JL, Favier F, Cunin F et al (1998) Crystalline and molecular structures of anhydrous lanthanide perchlorates Ln(ClO4)3 with Ln ¼ La, Ce, Pr, Sm, Eu, Ho, Er, Tm, and Lu. J Solid State Chem 139:259–265 81. Favier F, Pascal JL, Cunin F (1998) Thermal behavior and X-ray powder diffraction structures of two polymorphic phases of anhydrous Yb(ClO4)3. Inorg Chem 37:1776–1780 82. Blatov VA (2004) Voronoi-Dirichlet polyhedra in crystal chemistry: theory and applications. Cryst Rev 10:249–318 83. Conway JH, Sloane NJA (1988) Sphere packings, lattices and groups. Springer, New York 84. Arlt T, Armbruster T, Miletich R et al (1998) High pressure single-crystal synthesis, structure and compressibility of the garnet Mn3 2+ Mn2 3+ (SiO4)3. Phys Chem Miner 26:100–106 85. Weil M (2004) Fe3 II Fe4 III (AsO4)6, the ﬁrst arsenate adopting the Fe7(PO4)6 structure type. Acta Crystallogr E 60:i139–i141 86. Peskov MV, Blatov VA (2004) Comparative crystal-chemical analysis of binary compounds and d-metal halides containing tetrahedral anions. Russ J Inorg Chem 49:1042–1050 66 V.A. Blatov

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment